塑料名称LDPEHDPE乙丙共聚PPPP玻纤增强PPPSHIPSABS高抗冲ABS耐热ABS电镀级ABS阻燃ABS透明ABSACSAS(SAN)PMMA注塑工艺条件1、注塑机类型螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式螺杆-线式2、螺杆 形式1111111111111111111111111111111111转速,r/min11130-60130-6030-60130-6030-6030-6030-6020-6020-5030-6020-3020-5020-303、喷嘴 形式111直通式直通式直通式直通式直通式直通式直通式直通式直通式直通式直通式直通式直通式直通式直通式温度℃11150-1801170-190180-19011160-170180-190190-200190-200190-210180-190190-200160-170180-190180-2004、料筒温度 前℃11180-19011180-200190-20011170-190200-210200-210200-220210-230190-200200-220170-180200-210180-210中℃11180-22011200-220210-220111170-190210-230210-230220-240230-250200-220220-240180-190210-230190-230后℃11140-16011160-170160-170111140-150180-200180-200190-200200-210170-190190-200160-170170-180180-2005、模具温度,℃30-4530-6050-7040-8070-901120-5050-7050-8060-8540-8050-7050-7050-6050-7040-806、注射压力,MPA1170-1001170-12090-1301160-10070-9070-12085-12070-12050-10070-10080-12080-12090-1207、保压压力,MPa140-50150-6040-50130-4050-7050-7050-8050-7030-6050-6040-5040-5040-608、注射时间,s12-512-52-511-33-53-53-52-43-52-42-52-52-59、保压时间,s115-60120-6015-40115-4015-3015-3015-3020-5015-3015-4015-3015-3020-4010、冷却时间,s115-60115-5015-40110-4015-3015-3015-3015-3010-3010-3015-3015-3020-4011、总周期,s140-140140-12040-100140-9040-7040-7040-7040-9030-7030-8040-7040-7050-9012、干燥 设备卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾卧式沸腾温度℃90-10090-100100-120100-120100-12090-10090-110100-110100-110100-110100-110100-110100-11011100-120时间,h<0.5<0.5<0.5<0.5<0.5<0.50.5-1.00.5-1.00.5-1.00.5-1.00.5-1.000.5-1.00.5-1.0111.0